HAL Id: hal-02294384
Submitted on 4 Oct 2019
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
)2F3 and Na3V2(PO4)2FO2 type materials
Jacob Olchowka, Long H. B. Nguyen, Thibault Broux, Paula Sanz Camacho,
Emmanuel Petit, François Fauth, Dany Carlier, Christian Masquelier,
To cite this version:
Jacob Olchowka, Long H. B. Nguyen, Thibault Broux, Paula Sanz Camacho, Emmanuel Petit, et
Aluminum substitution for vanadium in the Na3V2(PO4 )2F3 and Na3V2(PO4)2FO2 type
materials. Chemical Communications, Royal Society of Chemistry, 2019, 55 (78), pp.11719-11722.
Received 00th January 20xx, Accepted 00th January 20xx DOI: 10.1039/x0xx00000x
Aluminum substitution for vanadium in the Na3V2(PO4)2F3 and
Na3V2(PO4)2FO2 type materials
Jacob Olchowka a,d,e, Long H. B. Nguyen a,b,d, Thibault Broux a,b,d,e, Paula Sanz Camacho a,d, Emmanuel
Petit a,d,e, François Fauth c, Dany Carlier a,d,e, Christian Masquelier b,d,e Laurence Croguennec a,d,e,*
Among the positive electrode materials for Na-ion batteries, Na3V2(PO4)2F3 is considered as one of the most promising and generates high interest. Here, we study the influence of the sol-gel synthesis parameters on the structure and on the electrochemical signature of the partially substituted Na3V2-zAlz(PO4)2(F,O)3 materials. We demonstrate that the acidity of the starting solution influences the vanadium oxidation state of the final product. For the first time we report on the possibility of controlling the double Al/V and O/F substitution that leads to the preparation of the Na3V2-zAlz(PO4)2F1+zO2-z solid solution.
These last years the booming electric and hybrid vehicle market conjugated to the development of renewable energy technologies have generated a strong interest in alternative electrochemical storage technologies to the Li-ion batteries.1
Among them, Na-ion batteries are nowadays considered as a reliable and more eco-friendly alternative due to the high abundance of sodium widespread all over the Earth. Within the large panel of possible positive electrode materials, Na3V2(PO4)2F3 (NVPF) is among the most promising ones due to
its excellent stability upon long range electrochemical cycling and to its attractive high rate performances when coated with carbon that allows fast charge compared to the layered oxides NaxMO2 (M= transition metal).2–4 Moreover, the reversible
extraction of two sodium ions at a potential of ~3.7 V (1st Na+)
and 4.2 V (2nd Na+) vs. Na+/Na leads to an energy density
comparable to that of the commercial Li-ion batteries using LiFePO4 at the positive electrode (507 Wh/kg for NVPF versus
530 Wh/kg for LiFePO4).5 Currently, NVPF is used as a positive
electrode material by the start-up TIAMAT that develops and produces functional 18650 cells as Na-ion battery prototypes. Very recently, the attractiveness of NVPF increased even more
since Yan et al. demonstrated the possibility to increase the energy density of the full cell NVPF versus hard carbon of ~14% by extracting more than two Na+ at high potential and due to its
promising performances reported in aqueous systems.6,7
In order to explore the possibility of modifying the values of the redox couples involved in the insertion/de-insertion reactions and thus the potential, the transport properties and the capacity retention at high rates, different approaches were explored. Anionic substitution of oxygen for fluorine has a significant impact on the crystal structure and electrochemical properties of Na3V2(PO4)2F3-yOy.8–11 The richer the oxygen
content, the lower the average discharge voltage and thus the energy densities are. Similarly, the effect of cationic doping/substitution for vanadium was studied using for instance yttrium, manganese, lanthanum or titanium in order to improve the electronic conductivity and Na+ mobility.12–14
However, only few of these studies actually addressed the characterization of the composition and the structure of the materials as obtained, in relation with the electrochemical performance. Kosova et al. have demonstrated that Lanthanum substitution was in fact a surface modification effect by LaPO4.15
The group of Ceder has studied gallium and aluminium substitution for vanadium, with the aim to disrupt the charge and Na+ orderings within the lattice and thus lower the energy
barrier for the reversible extraction of the 3rd Na.16,17 Among the
different metals, aluminium drew our attention as Al is cheaper, lighter, more environmentally friendly than V and, as a non-electrochemically active element, could participate to the stabilization of the material upon cycling. Furthermore, the partial substitution of 0.5 Al3+ for V in Na3V3+2-zAlz(PO4)2F3 would
lead to an increase of ~3% of the theoretical gravimetric capacity for the reversible exchange of 2 Na+ ions, while keeping
the extraction of the third Na+ ion possible (i.e. for the exchange
of 3 e- or Na+ ions per 1.5 V3+ in the pristine material). Bianchini
et al. have reported an aluminium substitution for vanadium in NVPF limited to z = 0.3 (Na3V1.7Al0.3(PO4)2F3) through solid-state
reaction.16 However, a loss of reversible capacity was observed
for the substituted materials, as only the V3+/V4+ redox couple
appeared to be involved in the redox processes in the potential range of 2 - 4.5 V vs. Na+/Na. On the other hand, Lalère et al.
interestingly demonstrated that the V4+/V5+ redox couple could
a CNRS, Univ. Bordeaux, Bordeaux INP, ICMCB UMR 5026, F-33600, Pessac, France. b Laboratoire de Réactivité et de Chimie des Solides, CNRS-UMR# 7314, Université de Picardie Jules Verne, F-80039 Amiens Cedex 1, France.
c CELLS-ALBA synchrotron, E-08290 Cerdanyola del Vallès, Barcelona, Spain. d RS2E, Réseau Français sur le Stockage Electrochimique de l’Energie, FR CNRS 3459, F-80039 Amiens Cedex 1, France.
e ALISTORE-ERI European Research Institute, FR CNRS 3104, Amiens, F-80039 Cedex 1, France.
Electronic Supplementary Information (ESI) available: [details of any supplementary information available should be included here]. See DOI: 10.1039/x0xx00000x
COMMUNICATION Journal Name
2 | J. Name., 2012, 00, 1-3 This journal is © The Royal Society of Chemistry 20xx
be activated in the partially substituted NASICON Na3V1.5Al0.5(PO4)3 at an average voltage of 3.95 V vs Na+/Na.18
In order to increase the Al-content in the substituted phases, Na3V2-zAlz(PO4)2F3, we here employed a sol-gel synthesis
approach that allows a better chemical homogeneity of the precursors and leads to a higher material purity than through a traditional ceramic approach.19 We performed the synthesis in
acidic and basic media in order to study the effects of the pH on the crystal structure and onthe electrochemical performances
of the phases obtained.
For the synthesis of Na3V1.5Al0.5(PO4)2F3 in acidic medium
(NVPF-Al0.5-acidic), citric acid monohydrate, NH4VO3 and
Al(NO3)3.9H2O with an appropriate molar ratio 2 : 1.5 : 0.5 were
first dissolved in a Teflon beaker containing about 100 mL of H2O. Then, NH4H2PO4 and NaF (5% in excess), were successively
and slowly added to the solution. Once the solution turned green, which corresponded to the reduction of V5+ to V3+, it was
heated overnight at 80°C under continuous stirring, resulting in a beige/dark powder. This powder was finely ground, placed in a golden crucible, and heated at 350°C during 4h to eliminate the volatile species. The as-obtained powder was subjected to a second calcination at 650°C during 10h under continuous argon flow. Finally, the resulting black powder was washed in water to eliminate possible soluble impurities. The chemical composition of NVPF-Al0.5-acidic was confirmed by ICP-OES
(Inductively Coupled Plasma - optical emission spectrometry) with Na:V:Al:P cationic ratios of 3 : 1.5 : 0.5 : 2. Several attempts were made to further extend the Na3V2-zAlz(PO4)2F3
solid-solution at z values higher than z = 0.5, with limited success. Most of the time, a mixture of Na3V2(PO4)2F3, Na3Al2(PO4)2F3,
AlPO4 and NASICON-type Na3V2(PO4)3 were obtained. The
crystal structure of NVPF-Al0.5-acidic was determined by
Rietveld refinement using high-resolution synchrotron powder X-ray data (SXRD) from the ALBA synchrotron facility (see Figure
1a). As for NVPF,
NVPF-Al0.5-acidic presents a subtle orthorhombic distortion,
which is described in the Amam space group (see Figures 1a and S1-S2, Tables S1-S2).20 A shrinkage of the cell volume is
observed in the NVPF-Al0.5-acidic phase (862.65(1) Å3 vs.
877.54(1) Å3 for NVPF), which is due to the smaller ionic radius
of Al3+ vs. V3+ (respectively 0.535 Å and 0.64 Å in an octahedral
coordination) (see Table S3 and Figure 2a-b).
The use of NaF in acidic media may leads to HF release, which is a volatile species that can easily evaporate at 80°C. In order to minimize the possible departure of harmful HF during the evaporation step, which may be the cause of the formation of NASICON-type phases, the synthesis procedure was further modified by using a NH4OH (28-30% NH3 basis) buffer solution
to adjust the pH of the solution at ~9.2 during the dissolution process. By controlling the pH, the solution quickly turned into blue indicating the possible presence of V4+. Thanks to this
modified method, a new family of Al-substituted phases, Na3V 2-zAlz(PO4)2F1+zO2-z (0 ≤ z ≤ 2), was obtained (Figures S3-S4 and
Table S3). AlPO4 is present as an impurity in some samples;
however, this does not hinder the structural determination of the main phase by the use of Rietveld refinement. Figure 1b illustrates the SXRPD Rietveld refinement analysis of Na3V1.5Al0.5(PO4)2F1.5O1.5 synthesized in basic medium, called
NVPFO-Al0.5-basic. This phase crystallizes in the tetragonal P42/mnm space group. The reliability factors (RBragg = 4.5% and
Rwp = 10.4%) demonstrate the good quality of the Rietveld
refinement despite the presence of AlPO4 as a secondary phase
(up to ~12.1 wt.%) (Tables S4-S5). The cell parameters determined for the V4+-rich phase Na3V1.5Al0.5(PO4)2F1.5O1.5 are
a = 8.9593(1) Å and c = 10.5511(1) Å with a cell volume V = 846.93(1) Å3, significantly smaller than those reported for the
corresponding V3+-rich phase Na3V1.5Al0.5(PO4)2F3 (Table S3).
Elemental analysis performed by ICP-OES leads to a cationic ratio Na:V:Al:P of 3:1.5:0.5:2, which was shown to be the composition of the main NVPF-type phase despite the presence of AlPO4 as impurity. Indeed, this latter is sparsely soluble in HCl
solution, the acid used for the sample dissolution required to perform the chemical analyses (see supplementary information). Figure 2b shows a linear evolution of the cell parameter c (along the bioctahedral unit, see Figure 2a) for all the phases Na3V2-zAlz(PO4)2F1+zO2-z (0 ≤ z ≤ 2) implying a
solid-solution formation according to Vegard’s law. Interestingly, starting from the same V : Al ratio (V1.5Al0.5) and monitoring the
sol-gel synthesis conditions in acidic and basic media, two original materials could be obtained: Na3V3+1.5Al3+0.5(PO4)2F3 and
Na3V4+1.5Al3+0.5(PO4)2F1.5O1.5. The first composition maintains
the same structure as NVPF, with a small orthorhombic distortion (b/a ~ 1.002) and Na+ ions distributed among three
different sites in the tunnels, whereas the second one is also stabilized in a structure close to that of NVPF, but described in
Figure 1. Rietveld refinement of synchrotron powder X-ray diffraction data recorded at λ = 0.6202 Å for: a) NVPF-Al0.5-acidic refined in the Amam space group and b)
a tetragonal unit cell with only two sites for the Na+ ions. In
order to get more insight into the difference in cell parameters between NVPF-Al0.5-acidic and NVPFO-Al0.5-basic, the
environments of V (Al) in the two structures were compared, based on the structural determination performed by Rietveld refinement. The major difference was observed for the apical V/Al-(F,O) bond lengths along the bi-octahedral units (V,Al)2O8(F,O)3. As described in Figure 2c, the terminal V/Al-F
bonds of the bi-octahedra V1.5Al0.5O8F3 observed in
NVPF-Al0.5-acidic are of 1.928(2) Å which is in good accordance
with the common value found for a Al/V3+-F bond. On the other
hand, the terminal V/Al-O/F bond lengths are estimated to be of 1.654(3) Å in NVPFO-Al0.5-basic, which fits well with an
average distance corresponding to the contribution of 25% of
Al-F bonds close to 1.82 Å and of 75% of V4+=O vanadyl bonds
close to 1.6 Å.21
As oxygen and fluorine cannot be distinguished by X-ray diffraction and cannot be easily titrated by chemical analyses, analyses by Fourier Transformed Infrared (FTIR) and 31P
solid-state Nuclear Magnetic Resonance (ss-NMR) spectroscopies were performed and compared to those of Na3V3+2(PO4)2F3 and
Na3V4+2(PO4)2FO2 as reference compounds. The absence of
vibration bands characteristic of νV=O (vanadyl bond) at ~ 919
cm-1 in the IR spectrum of NVPF-Al0.5-acidic confirms that the
material contains only V3+ (Figure 3a) confirming the
Na3V3+1.5Al0.5(PO4)2F3 composition. Additionally, the 31P ss-NMR
spectrum of Na3V3+1.5Al0.5(PO4)2F3 exhibits 5 signals which can
be attributed to phosphorus surrounded by different numbers of V3+ in its first cationic coordination sphere (the signals at
~6000 ppm, ~4500 ppm, ~3000 ppm, ~1500 ppm and ~0 ppm are attributed to P(OV3+)
4, P(OV3+)3(OAl3+), P(OV3+)2(OAl3+)2,
P(OV3+)(OAl3+)3 and P(OAl3+)4 local environments, respectively).
Based on our 31P MAS NMR study of the Na3V3+2-yV4+y(PO4)2F 3-yOy phases, a V3+ octahedra sharing a corner with PO4
tetrahedra results in a Fermi contact interaction of about 1500 ppm, whereas a V4+ one do not lead to any shift
contribution.8 Here, a Al3+ ion that does not possess unpaired
electrons does not contribute to any Fermi contact shift and thus behave similarly as a V4+ ions in the lattice. Based on the
relative signal intensities, the Al3+/V3+ ionic distribution in the
material is close to the statistical one. On the other hand, as for the reference Na3V4+2(PO4)2FO2 (blue spectrum), NVPFO-Al0.5
-basic (green spectrum) displays only a diamagnetic signal at ~0 ppm (see Figure 3b). This observation confirms the absence of V3+ in the structure. Concomitantly, the FTIR spectrum of
NVPFO-Al0.5-basic exhibits intense bands centred at ~925 cm-1
and its overtone at 1850 cm-1 revealing the presence of vanadyl
bonds and hence, V4+ in the structure, which confirms the
Na3V4+1.5Al0.5(PO4)2F1.5O1.5 formula (see Figure 3a).22
The electrochemical signatures of the Na3V3+1.5Al0.5(PO4)2F3
and Na3V4+1.5Al0.5(PO4)2F1.5O1.5 were studied in half cells vs. Na
and compared to those of Na3V3+2(PO4)2F3 (carbon-coated) and
Na3V4+2(PO4)2FO2. Figure 4a displays the charge/discharge data
of the four materials in the potential range 2.8 - 4.5 V vs. Na+/Na
and at a cycling rate of C/10 per Na+. For Na3V3+1.5Al0.5(PO4)2F3,
the charge is characterized by two “sloping plateaus” at average potentials of 3.69 V and 4.23 V vs. Na+/Na, which respectively
correspond to the extraction of 1 and 0.5 Na+. The polarization
is much greater than for NVPF, as more extensively discussed in the supplementary information, and the “plateaus” are more sloping as indicated by the broad peaks observed on the first derivative data (see Figure 4b). The high polarization induces
Figure 2. a) Representation of the Na3(V,Al)2(PO4)2(F,O)3 crystal structure; b) Evolution of the c unit cell parameter of Al-substituted Na3V2-zAlz(PO4)2(F,O)3 phases as a function of
the aluminium content; c-d) Description of the vanadium/aluminium bi-octahedra in Na3V3+1.5Al3+0.5(PO4)2F3 (NVPF-Al0.5-acidic) and Na3V4+1.5Al3+0.5(PO4)2F1.5O1.5 (NVPFO-Al0.5-basic).
Figure 3. a) FTIR spectra of (red spectrum) assigned to be
Na3V1.5Al0.5(PO4)2F3, Na3V2(PO4)2F3 (black spectrum (green
spectrum) assigned to be Na3V1.5Al0.5(PO4)2F1.5O1.5, and Na3V2(PO4)2FO2 (blue spectrum)
recorded in the wavenumber range 400 – 1990 cm-1 b) 31P ss-NMR spectra of NVPF-Al0.5
-acid (red spectrum), Na3V2(PO4)2F3 (black spectrum), NVPFO-Al0.5-basic (green
spectrum), and Na3V2(PO4)2FO2 (blue spectrum) recorded at 100 MHz, MAS = 30 kHz
COMMUNICATION Journal Name
4 | J. Name., 2012, 00, 1-3 This journal is © The Royal Society of Chemistry 20xx
significant capacity loss between the charge and discharge and the sloping “plateaus” reveal a solid-solution type mechanism upon insertion and desinsertion of Na+ whereas intermediate
phases and biphasic domains are observed for NVPF. The extraction of 1.5 Na+ suggests that only the V3+/V4+ redox couple
can be activated in the electrolyte stability window (up to 4.5 V vs. Na+/Na) and the structural distortion in the bioctahedra
induced by V/Al substitution does not allow the activation of the V4+/V5+ redox couple in this potential range. The extra-capacity
obtained at high potential (> 4.5 V vs. Na+/Na) (Figure S5) is not
completely reversible and is discussed in the supplementary part S5).
The electrochemical signature of Na3V4+1.5Al0.5(PO4)2F1.5O1.5
is also characterized by two “plateaus” corresponding to the reversible extraction of ~1 Na+ and 0.5 Na+ at average potentials
of ~3.66 and 4.05 V vs. Na+/Na respectively. Compared to
Na3V4+2(PO4)2FO2, the Na+ extraction voltage in
Na3V4+1.5Al0.5(PO4)2F1.5O1.5 is not affected by the Al-substitution.
However, the polarization increases significantly leading to a reduction in the efficiency of the electrode material. The reversible extraction of 1.5 Na+ shows that the (V=O)2+/(V=O)3+
redox couple (or V4+/V5+ with V engaged in vanadyl bonds) could
be activated, on the contrary to the V4+/V5+ engaged in V-F
bonds. For Na3V4+1.5Al0.5(PO4)2F1.5O1.5, the theoretical capacity is
To summarize, we succeeded to synthesize a highly substituted (Al for V) range of compositions in the Na3V3+1.5Al0.5(PO4)2F3 solid-solution and reported for the first
time the controlled synthesis of a series of combined anionic and cationic substituted positive electrode materials of general formula: Na3V4+2-zAlz(PO4)2F1+zO2-z (0 < z < 2). The Al for V
substitution has a minor effect on the average potential of the Na+ extraction, on the contrary to F/O substitution that strongly
lowers the extraction potential of the high voltage plateau (2nd Na+). For Na3V3+1.5Al0.5(PO4)2F3, although the V/Al partial
substitution increases the theoretical gravimetric capacity, only the V3+/V4+ redox couple could be activated in the potential
range 2.8 - 4.5 V vs. Na+/Na which lowers the specific energy.
On the other hand, the theoretical capacity is reached for Na3V4+1.5Al0.5(PO4)2F1.5O1.5. These results confirm also that the
(V=O)2+/(V=O)3+ redox couple (or V4+/V5+ with V engaged in
vanadyl bonds) could be reversibly activated in the stability window of current electrolytes, on the contrary to the V4+/V5+
engaged in V-F bonds. These solid solutions call to be scrutinized much more in details to determine the substitution in Al and O just sufficient to optimize the properties of the very attractive electrode material for Na-ion batteries, Na3V2(PO4)2F3, the panel of properties
being well beyond the reversible capacity only. Indeed, the chemical and thermal stability in the charge state of the battery is for instance one of them, as controlling the safety of the battery but also the long range cyclability.
The authors thank the RS2E and Alistore-ERI Networks for the funding of LHBN’s PhD thesis and TB’s postdoctoral fellowship, as well as the financial support of Région Nouvelle Aquitaine, of the French National Research Agency (STORE-EX Labex Project ANR-10-LABX-76-01 and SODIUM Descartes project ANR-13-DESC-0001-02) and of H2020 research and innovation program under the Grant Agreement No. 646433-NAIADES. The authors also want to thank C.DENAGE, A. FARGUES and E.LEBRAUD (ICMCB) for their help with SEM, FTIR and XRD analyses, respectively.
Conflicts of interest
There are no conflicts of interest to declare.
Notes and references
1 D. Larcher and J. M. Tarascon, Nat. Chem., 2015, 7, 19–29. 2 T. Broux, F. Fauth, N. Hall, Y. Chatillon, M. Bianchini, T. Bamine, J.-B. Leriche, E. Suard, D. Carlier, Y. Reynier, L. Simonin, C. Masquelier and L. Croguennec, Small Methods, 2018, 2, 1800215.
3 C. Zhu, C. Wu, C. C. Chen, P. Kopold, P. A. Van Aken, J. Maier and Y. Yu,
Chem. Mater., 2017, 29, 5207–5215.
4 C. Masquelier and L. Croguennec, Chem. Rev., 2013, 113, 6552–6591. 5 B. Senthilkumar, C. Murugesan, L. Sharma, S. Lochab and P. Barpanda,
Small Methods, 2018, 3, 1800253.
6 G. Yan, S. Mariyappan, G. Rousse, Q. Jacquet, M. Deschamps, R. David, B. Mirvaux, J. W. Freeland and J.-M. Tarascon, Nat. Commun., 2019, 10, 585. 7 P. R. Kumar, Y. H. Jung, C. H. Lim and D. K. Kim, J. Mater. Chem. A, 2015,
8 T. Broux, T. Bamine, F. Fauth, L. Simonelli, W. Olszewski, C. Marini, M. Ménétrier, D. Carlier, C. Masquelier and L. Croguennec, Chem. Mater., 2016,
9 P. Serras, V. Palomares, J. Alonso, N. Sharma, J. M. López Del Amo, P. Kubiak, M. L. Fdez-Gubieda and T. Rojo, Chem. Mater., 2013, 25, 4917–4925. 10 Y. U. Park, D. H. Seo, H. S. Kwon, B. Kim, J. Kim, H. Kim, I. Kim, H. I. Yoo and K. Kang, J. Am. Chem. Soc., 2013, 135, 13870–13878.
11 L. H. B. Nguyen, T. Broux, P. S. Camacho, D. Denux, L. Bourgeois, S. Belin, A. Iadecola, F. Fauth, D. Carlier, J. Olchowka, C. Masquelier and L. Croguennec, Energy Storage Mater., 2019, 20, 324–334.
12 W. Liu, H. Yi, Q. Zheng, X. Li and H. Zhang, J. Mater. Chem. A, 2017, 5, 10928–10935.
13 H. Yi, M. Ling, W. Xu, X. Li, Q. Zheng and H. Zhang, Nano Energy, 2018,
14 Y. Zhang, S. Guo and H. Xu, J. Mater. Chem. A, 2018, 6, 4525–4534. 15 N. Kosova, D. Rezepova and N. Montroussier, Batteries, 2018, 4, 32. 16 M. Bianchini, P. Xiao, Y. Wang and G. Ceder, Adv. Energy Mater., 2017,
17 I. L. Matts, S. Dacek, T. K. Pietrzak, R. Malik and G. Ceder, Chem. Mater., 2015, 27, 6008–6015.
18 F. Lalère, V. Seznec, M. Courty, R. David, J. N. Chotard and C. Masquelier, J. Mater. Chem. A, 2015, 3, 16198–16205.
19 A. E. Danks, S. R. Hall and Z. Schnepp, Mater. Horiz., 2016, 3, 91–112. 20 M. Bianchini, N. Brisset, F. Fauth, F. Weill, E. Elkaim, E. Suard, C. Masquelier and L. Croguennec, Chem. Mater., 2014, 26, 4238–4247. 21 J. Le Meins and G. Courbion, J. Solid State Chem., 1999, 148, 260–277.
Figure 4 a) Charge/discharge galvanostatic data for Na3V1.5Al0.5(PO4)2F3, Na3V2(PO4)2F3,
Na3V1.5Al0.5(PO4)2F1.5O1.5 , and Na3V2(PO4)2FO2 at a cycling rate of C/10 per Na+. The
materials were cycled versus Na metal in 1M NaPF6 in EC : DMC = 1 : 1 with 2 wt.% of
22 Y. Qi, L. Mu, J. Zhao, Y. S. Hu, H. Liu and S. Dai, Angew. Chemie - Int. Ed., 2015, 54, 9911–9916.